Fabrication of reduced graphene oxide/chitosan composite fiber by dry-jet wet spinning
- 376 Downloads
Reduced graphene oxide (rGO) which was nontoxic, reduced from graphene oxide (GO), and decorated was mixed with chitosan (CS) solution to prepare rGO/chitosan (rGO/CS) biocomposite fiber by dry-jet wet spinning. rGO-/genipin-cross-linked CS (rGO/GCS) composite fiber was prepared. The conditions on nontoxic reduction of GO, namely decoration, spinning, drawing, and nontoxic cross-linking, were studied and optimized. The way to disperse rGO homogeneously in spinning solution was discussed. After surface decorating, rGO was covered by CS without reunion. No phase separation in rGO/CS spinning solution was observed. The solution remained stable for a week after being diluted. The decoration of CS was an effective way to achieve homogeneous dispersion of rGO in solution for spinning. Raman spectroscopy, Fourier-transform infrared spectroscopy (FTIR), X-ray diffraction (XRD), scanning electron microscope (SEM), transmission electron microscopy (TEM), and fluorescence spectroscopy were used to characterize the fibers and their precursors. A series of rGO/CS fibers with a diameter of 0.1 mm were successfully fabricated. The well-dispersed and exfoliated rGO nanosheets were assembled in CS matrix. Both rGO/CS fibers and rGO/GCS fibers maintained the intrinsic fluorescence. Both uncross-linked and cross-linked composite fibers could be bent freely. The work built up the foundation for systematic conductivity and mechanical property research about rGO/CS composite fibers.
KeywordsGraphene oxide (GO) Reduced graphene oxide (rGO) Chitosan (CS) rGO-/genipin-cross-linked CS (rGO/GCS) Composite fiber
Biodegradable scaffold materials play important roles in nerve transplantation. Scaffold material and seed cells constitute the core of 3D network of tissue engineering. There are certain requirements for scaffold materials, including the following: (1) good biocompatibility, scaffold materials should be nontoxic to cells; (2) good mechanical properties, to meet the needs of operating and supporting cells; (3) controllable biodegradability; and (4) electrical conductivity. Electrical stimulation has been proved to be effective in promoting adhesion, growth, directional differentiation, and the migration of stem cells by clinic studies, which is significantly important to improve remediation. For this purpose, the scaffold material should be electrically conductive. It is extremely challenging for material science and engineering to meet all above requirements [1, 2, 3, 4, 5, 6]. Chitosan (CS), a natural macromolecule which is abundant in the chitin shells of shrimp and other crustaceans, is biodegradable, nontoxic, and antibacterial [7, 8, 9, 10, 11, 12, 13]. In medicine, it may be useful in bandages to reduce bleeding and as an antibacterial agent; it can also be used to help deliver drugs through the skin. However, the relatively poor mechanical properties and electrical insulation of CS strongly restrict its usages as scaffold materials. Here, we propose a strategy to overcome those shortcomings by incorporating graphene (GN) in CS fiber.
GN has extraordinary mechanical and excellent electronic properties and good biocompatibility [14, 15]. Usually, GN is produced by reduction of graphene oxide (GO). Recently, GO has shown great promise for biomedical applications, such as cell imaging and biosensors. With abundant hydrophilic functional groups, such as −COOH and –OH, GO has strong van der Waal interactions with polymers, especially hydrophilic polymers. It is easy to disperse GO in aqueous and some organic solvents. Many studies on GO/CS composites have demonstrated that GO was an efficient nanofiller for reinforcing CS to achieve better mechanical properties without conductivity. Although some GO-reinforced CS materials were claimed to be potentially useful as biomaterials, so far, little work on GN/CS composite has been reported due to its incompatibility and etc. [16, 17, 18, 19, 20, 21, 22, 23, 24, 25, 26, 27, 28, 29, 30, 31, 32, 33, 34, 35, 36, 37].
For the reduction of GO to GN, hydrazine, which is toxic, is the most commonly used reducing agent. A nontoxic reduction is important for the application of GN in the field of biomaterials. Here, nontoxic ascorbic acid (LAA) was chosen to be the reducing agent. After reduction, GO lost most –OH and –COOH functional groups, and the formed GN has weak interfacial interaction with polymers. A surface decoration with nontoxic conjugate structure on GN is important to improve its interactions with polymers.
A great deal of reports on electrospun fiber has been published. Electrospun fibers usually have small diameters from a few nanometers to hundreds of nanometers. However, the poor orientation of electrospun fiber makes it difficult to obtain strong fiber for 3D braiding and inconvenient for stem cell to adhere. In comparison, highly drawn fibers of large diameters (from a few micrometers to a few millimeters) could be obtained by dry-jet wet spinning, which promotes the orientation of polymer chains and GN and improves the mechanical and conductive properties of the resulting fiber. Dry-jet wet spun fiber can be woven into a 3D scaffold with controllable patterns and good mechanical performance. The 3D scaffold can be designed and knitted according to damaged nerves, which provides a microenvironment suitable for the orientated growth of stem cells.
Mechanical properties and the degradation speed of CS fibers and its scaffold can be adjusted by cross-linking and braiding structure during post-drawing process [8, 9, 10, 11, 12, 13]. Instead of glyoxal, a common cross-linking agent for CS, a nontoxic cross-linking reagent genipin extracted from gardenia fruit was used in this study. So, in this work, we try to make some progress towards preparing biodegradable scaffold fiber for 3D braiding, which is nontoxic, electrically conductive, and available for mass production in a cheaper way.
CS (deacetylation rate 85%, viscosity 800~1000 mPa/s) was purchased from Huantai Jinhu Crust Co. Ltd., GO aqueous solution was obtained from Leadernano Tech L. L. C (Jining, China). Genipin was provided by Linchuan Zhixin BioTechnology Co, Ltd (Jiangxi, China). Ascorbic acid (LAA) was purchased from Beijing Chemical Reagent Co, Ltd. Other reagents were bought from Sinopharm Chemical Reagent Co, Ltd (Shanghai, China).
2.2 Experimental methods
2.2.1 Nontoxic reduction of GO and nontoxic decoration of rGO
During the reduction of GO, the functional groups on GO surface continue to decrease; the hydrophobic increases, leading to agglomerating. How to keep a stable dispersion of rGO is very important to prepare spinning solution.
Ordinary decoration of GN (surface-active agent, grafting functional groups, radiation, etc.) helps to form strong interaction between CS and GN and to improve the strength of the composite fibers. For our purpose, the surface decoration must be nontoxic without significantly damaging conjugate structure of GN. Thus, we used CS itself as surface treatment agent and GN stabilizer.
A mixture of 0.4 g GO (aqueous solution of 5 mg/l) and 3.75 g LAA reacted for 6 h at 60 °C, then LAA was washed off. CS and acetic acid (HAc) solutions were added followed by ultrasonication for 30 min using a pulsed horn sonicator. The pH value was adjusted to 7 by NaOH for rGO decoration and then ultrasonicated for 1.5 h until the solution became homogeneous.
3.8% CS powder and 2% HAc, various amounts of decorated rGO solution, and distilled water were mixed together in a flask equipped with an overhead mechanical stirrer and were stirred for 4 h at room temperature to obtain spinning solutions. (All ratios described in the text refer to weight ratio.) By changing the weight fraction of the decorated rGO in CS from 1.1 to 2 to 9% etc., a series of spinning solution, referred as 1.1% rGO/CS, 2% rGO/CS, 9% rGO/CS, etc., was prepared.
2.2.2 Spinning and drawing
After filtering and defoaming, spinning solution was transferred into an extruder. The spinning solution was extruded through an air gap of 3 cm and entered a coagulation bath within a solution of 105 g NaOH, 2 l ethanol (95%), and 1.9 l water. Then, the nascent fiber was washed by passing through a methanol bath at room temperature to remove water. The as-spun fiber was hot drawn in multiple stages by passing through hot water at 60 and at 80 °C, respectively. rGO/CS composite fiber without cross-linking was obtained.
2.2.3 Preparation of genipin-cross-linked rGO/CS composite fiber
The drawn fiber was dipped in the solution of 100 μL genipin (50 mg/ml in ethanol) and incubated for 12 h at 30 °C. The cross-linked fiber was rinsed and dried under vacuum at 40 °C for 48 h.
FTIR spectra were recorded using an IR spectroscopy (Spectrum 100, PerkinElmer). Raman was carried on LabRAM HR Evolution with an excitation wavelength of 532 nm. The morphologies of the rGO/CS composite fiber were imaged using a SEM (Hitachi S-4800). Samples for cross-sectional view were obtained by tensile fracture in liquid nitrogen. Morphologies of rGO in composite fiber were imaged using a TEM (FEI TECNAI G2 F30). The structure of the cross-linked and uncross-linked rGO/CS fibers was characterized and compared by using X-ray diffraction (XRD-3, Peking University, 40KV, 16 mA, with a Cu rotating anode parallel focused X-ray source of 1.5418 Å). Fluorescence study was carried out on inverted fluorescence microscopy (LEICA, DMI 6000B).The tensile strength test was on CMT4304, XinSanSi Co. China (which now belongs to MTS Systems Corporation, USA). The electrical resistivity of rGO/CS composite fibers was measured with UT56 Multimeter (UNI-T).
4 Results and discussion
4.1 Nontoxic reduction of GO and nontoxic decoration of rGO
In aqueous solution, along with the reduction of GO, its hydrophobicity increased, leading to agglomeration. In order to keep the stable dispersion of rGO, both the reduction agent and stabilizer agent were simultaneously used during the chemical treatment of rGO.
Owing to the strong intrinsic van der Waals forces, nano-sized rGOs always aggregate in most solvents. Even though the rGO/CS blends have been sonicated before surface deposition, rGO still has a strong tendency to form bundles. Chitosan is a linear polysaccharide composed of randomly distributed β-(1→4)-linked D-glucosamine (deacetylated unit) and N-acetyl-D-glucosamine (acetylated unit). Along with the increase of pH, the ionized CS will be deionized and become non-dissolvable in aqueous media. Then, the CS deposits on rGO and forms a CS shell. The interaction between CS and rGO is expected to be strong. Electrostatic attraction among rGO sheets becomes weak after the surface decoration. This is due to the static-repellency of the CS shell. Without the decoration, rGO coagulates even in CS solution.
Combining the properties of rGO and the versatility and biocompatibility of CS, these CS surface-decorated rGO may have broad applications.
4.2 Dry-jet wet spinning and hot drawing
The air gap between spinneret and coagulating bath played an important role for the formation of as-spun fiber. If the dope thread was positively drawn (draw ratio > 1), the orientation of chain segments created inside nozzle channel by shear stress would be strengthened in the air gap; as a result, the fiber tenacity would be expected to increase, whereas if the dope thread was negatively drawn (draw ratio < 1), the shear orientation created during nozzle channel would be relaxed in the air gap and then the fiber tenacity would be expected to decrease. The optimal operation parameter values for continuous and stable spinning process are as follows: a spinning speed of 1–3 ml/min, spinneret diameter of 0.86 mm, and reeling velocity of 1–7 m/min.
When temperature of drawing bath increased, the mobility of macromolecules is strengthened and the inner solvent is driven out more easily; thus, the draw ratio and fiber tenacity are increased, but the effect of temperature tends to be leveled off as the temperature reaches above 80 °C. At last, uniform fibers have been obtained (as shown in Fig. 4b).
4.3 Nontoxic cross-linking of rGO/CS composite fiber
4.4 Fluorescence study
The well-dispersed rGO sheets divide the large conjugated groups into smaller ones. Thus, the fluorescence intensity of the composite fibers decreases along with the increase of rGO loading. On the other hand, rGO sheets quench the intensity of the excitation light. Although fluorescence intensity reduced, rGO-incorporated samples are still highly visible. This fluorescent property of rGO/GCS exhibits advantages for biomedical and bioimaging applications. Degradation of rGO/GCS scaffold may be investigated outside body in future.
4.5 Mechanical properties and electron conduction
After surface decorating, rGO is covered by CS without reunion. There is no visible phase separation in rGO/CS spinning solution. The solution is stable after being diluted even after a week. The decoration of CS is an effective way to achieve homogeneous dispersion of rGO in solution for spinning. A series of rGO/CS fibers with a diameter of 0.1 mm has fabricated by a dry-jet wet spinning successfully. A better process condition has been obtained. The well-dispersed and exfoliated rGO nanosheets are assembled in CS matrix. Both rGO/CS fibers and rGO/GCS fibers maintain the intrinsic fluorescence. Both uncross-linked and cross-linked composite fibers can be bent freely. The work lays the foundation for further research on other properties of rGO/CS composite fibers.
This work was supported by the Fundamental Research Funds for the Central Universities (no. 53200859721 and no.2-9-2017-346) and the Innovation and Entrepreneurship Training Project for Undergraduate Students (2016AX031), China University of Geosciences, Beijing.
Compliance with ethical standards
Conflict of interest
The authors declare that they have no conflict of interest.
- 13.Wang G, Zheng L, Zhao H, Miao J, Sun C, Ren N, Wang J, Liu H, Tao X (2011) In vitro assessment of the differentiation potential of bone marrow-derived mesenchymal stem cells on genipin-chitosan conjugation scaffold with surface hydroxyapatite nanostructure for bone tissue engineering. Tissue Eng Part A 17:1341–1349CrossRefGoogle Scholar